- Email: [email protected]

Contents lists available at ScienceDirect

Computational Materials Science journal homepage: www.elsevier.com/locate/commatsci

Magnetic properties of NiCl2 nanostructures A.N. Enyashin, A.L. Ivanovskii * Institute of Solid State Chemistry, Ural Branch of the Russian Academy of Sciences, 620990 Ekaterinburg, Russia

a r t i c l e

i n f o

Article history: Received 31 May 2010 Received in revised form 10 June 2010 Accepted 10 June 2010 Available online 6 July 2010 Keywords: NiCl2 Nanostructures Magnetic properties Simulations

a b s t r a c t We show that the magnetic properties of antiferromagnetic layered NiCl2 can be altered under nanosizing depending on dimensionality and morphology type of the corresponding nano-forms. By means of Monte-Carlo simulations within classical Heisenberg model, the spin ordering, magnetic part of heat capacity Cv and Néel temperatures TN for multi-walled NiCl2 nanotubes and a fullerene were calculated and analyzed in comparison with the bulk NiCl2 and multilayered two-dimensional NiCl2 crystals and nanostripes. We have found that the nanostructuring of NiCl2 at the size reducing and at the formation of the closed structures can inﬂuence propitiously on the preservation of antiferromagnetic properties and the suppression of superparamagnetic limit. Ó 2010 Elsevier B.V. All rights reserved.

1. Introduction Among the magnetic materials suitable for a wide range of practical applications, quasi-two-dimensional antiferromagnetic systems have attracted interest. The well known representatives of these systems are dihalides of d-metals with CdCl2 structural type [1], for example, nickel dichloride NiCl2 [2]. In the ground state, NiCl2 contains ferromagnetic layers of nickel ions, which are antiferromagnetically ordered among themselves and in a weak magnetic ﬁeld undergo the transition from antiferromagnetic phase to ferromagnetic phase [3,4]. In the last 5 years appreciable results have been achieved in the preparation of a wide group of nanosized d-metal dihalides (NiCl2, FeCl2, CdCl2, CdI2, NiBr2) with morphology of nanotubes, octahedral fullerenes and fullerene-like nanoparticles by laser, electron beam or thermal evaporation and condensation [5–11]. However, there are no reliable data on the electronic and magnetic properties of these nanostructures, because they appear as a mess of particles with different size and morphology, which are unstable against humid atmosphere. It prevents from a massive and expedient production of nanostructured halides and explains a poor characterization of hollow halide nanostructures to date. Recent experiments on capillary imbibition of molten PbI2 by WS2 nanotubes have resulted in the preparation of core–shell [email protected] nanotubes [12], which shows a direction for guided production of protected and well crystallized halide nanotubes with more or less a uniform size, depending only on the size of the chalcogenide nanotubes [13]. The diameters of chalcogenide nanotubes

* Corresponding author. E-mail address: [email protected] (A.L. Ivanovskii). 0927-0256/$ - see front matter Ó 2010 Elsevier B.V. All rights reserved. doi:10.1016/j.commatsci.2010.06.023

are typically an order of magnitude larger than the diameters of carbon nanotubes [14], and the ﬁnal product after capillary imbibition and cooling of molten PbI2 within WS2 nanotubes may differ from bulk nanocrystallites, since the strain energy of PbI2 monolayer adsorbed on WS2 surface will be not a limiting factor for a formation of rolled PbI2 structures. The formation of multiwall nanotubes of layered PbI2 coaxial to the WS2 nanotubes can be easily observed [12,15]. It opens new horizons in the guided fabrication of nanostructures of related halides, since the capillary ﬁlling of chalcogenide nanotubes can offer in a nearest future the production of protected and well crystallized halide nanostructures with more or less uniform size and permanent electronic and magnetic properties, depending only on the size distribution of the chalcogenide nanotubes [16]. In this work we present preliminary results about a possible inﬂuence of nanostructuring on the magnetic properties of NiCl2. Using Monte-Carlo simulations within framework of classical Heisenberg model the spin ordering, magnetic part of heat capacity Cv and Néel temperatures TN for multi-walled NiCl2 nanotubes and a fullerene were calculated in comparison with the bulk NiCl2 and corresponding multilayered two-dimensional NiCl2 crystals and nanostripes. 2. Structure models and computational method 2.1. Models of NiCl2 nanostripes, nanotubes and fullerenes NiCl2 adopt layered CdCl2-type structure (space group R-3m, No. 16, Z = 3), where each Ni ion is coordinated by six Cl ions, and each Cl ion is bonded to three Ni centers [3,17]. For a description of antiferromagnetic state of the bulk NiCl2 we have used rectangular

783

A.N. Enyashin, A.L. Ivanovskii / Computational Materials Science 49 (2010) 782–786

supercell constructed from hexagonal unit cell with the parameters a = 3.468 Å and c = 34.40 Å, which contained six layers. Such model was used also for the simulation of the bulk material and two-dimensional double-, triple- and six-layered NiCl2 crystals and corresponding one-dimensional NiCl2 nanostripes, which supercells contained in general 2880 Ni atoms, see Fig. 1. Architecture of nanotubes, which are based on hexagonal NiCl2 monolayer, can be characterized within framework of the same classiﬁcation like for carbon and other related inorganic nanotubes [18,19]. Among single-walled nanotubes three types of chirality can be distinguished: zigzag (n,0), armchair (n,n) and chiral (n,m), with m – n and m – 0. Here we consider multi-walled nanotubes as a system of coaxial single-walled nanotubes. In spite of many other layered compounds (like graphite, MoS2, WS2, etc.) the perfect matching between lattice parameters a and c of the bulk NiCl2 gives a unique opportunity for the existence of nanotubes with the same interwall distance as van der Waals’ gap in the bulk material, i.e., the difference between chiral indexes for two adjacent armchair nanotubes Dn will have exact integer value calculated using p ﬃﬃ c ¼ 6:00. In general, we have considered three relation Dn ¼ 3p 3 a multi-walled nanotubes with the same outer diameter 95.6 Å: double- (44,44)@(50,50), triple- (38,38)@(44,44)@(50,50) and sixwalled (20,20)@(26,26)@(32,32)@(38,38)@(44,44)@(50,50), which

are composed by 10 unit cells and contained 1880, 2640 and 4200 Ni atoms, respectively. The models for NiCl2 fullerenes can be created in a similar way as for other inorganic layered compounds with MX2 stoichiometry [20,21]. This procedure includes the change in the evenness of M–X cycles. Namely, an introducing of six four-membered cycles (square-like defects) may result in the construction of octahedral particles as observed in experiments [5,6]. Triangular facetes of these octahedral nanoparticles are composed by the fragments of NiCl2 monolayer, while at the corners square-like defects are placed. In our work we have considered double-walled nanooctahedron (NiCl2)[email protected](NiCl2)3136 containing 5440 Ni atoms.

2.2. Computational details As a starting point of our method, classical Heisenbergs model has been applied. Hamiltonian for magnetic NiCl2 in the absence of magnetic ﬁeld may be written in the form [3]:

H¼

X i>j

2J ij Si Sj

X i>j0

2J 0ij0 Si Sj0 D

X i

2

Sxi D0

X y2 2 ðSi Szi Þ; i

ð1Þ

Fig. 1. Structures of the bulk NiCl2 (1), inﬁnite NiCl2 bilayer (2), one-dimensional (12,12) NiCl2 nanostripe (3), double-walled (44,44)@(50,50) NiCl2 nanotube (4) and fullerene (NiCl2)[email protected](NiCl2)3136 (5). Nickel atoms are only shown.

784

A.N. Enyashin, A.L. Ivanovskii / Computational Materials Science 49 (2010) 782–786

where Jij and J0ij are exchange integrals for inter- and intralayer spin interactions (Jij is equal 21.70 K and 4.85 K for the ﬁrst and second coordination spheres, respectively, J0ij = 0.77 K), D and D0 are constants of plane anisotropy (D = D0 = 0.40 K), Si ðSxi ; Syi ; Szi Þ is classical spin (with modulus equal 1). Aforementioned fact of perfect matching between a and c lattice parameters and equality of interlayer distances as well as intralayer interatomic distances both in the bulk and nanotubular NiCl2 allow to use the same values of Jij and J 0ij without a considerable correction for the distance between the spins. Thermodynamical properties of crystalline and nanostructured allotropes of NiCl2 were calculated using Monte-Carlo method (MC) applying Metropolis algorithm [22]. For every spin 5 104 MC steps were performed, at that ﬁrst 3 104 MC steps were used for thermalization, while the rest steps were intended for the calculation of magnetic part in molar heat capacity Cv using statistical ﬂuctuations of total energy E at temperature T as:

Cv ¼

1 kT

2

ðhE2 i hEi2 Þ:

ð2Þ

3. Results and discussion First, the simulation was performed for the bulk NiCl2 in order to estimate an error in the calculation of the magnetic ordering temperature TN (Néel temperature). The calculated dependence

of magnetic part of molar heat capacity Cv on temperature T demonstrates clear peak at T = 63 K which corresponds to a phase transition (Fig. 2) and may be attributed to TN. An analysis of the spin ordering depending on the temperature proves this supposition (Fig. 3). At T > 63 K the spin ordering is lost, and the magnetic structure of a layer within the bulk is represented by the ‘‘islands” of Ni ions with different spin orientation, while at T < 63 K the magnetic structure is represented as a classical antiferromagnetic system composed by layers with alternating spin orientation along c-axis. Thus, the use of the above mentioned values of exchange integrals for inter- and intralayer spin interactions [3] leads to an overestimation of TN on 10.7 K in comparison with experimental data TN = 52.3 K [3]. Therefore, their use in further simulations of magnetic properties of NiCl2 systems can provide a semi-quantitative estimation. Let us note that the origin of second low-intensity peak of Cv at T = 25 K is not clear and its existence has not been reported in the past [2]. Based on the results of our MC simulations, we may suppose that this peak is related to partial low-temperature change of the spin orientations: at temperatures below 25 K a kind of spin waves is obtained across c-axis of the crystal, which disappears at higher temperatures. Though, this phenomenon may be an artifact of the model applied, when classical Heisenbergs Hamiltonian (1) fails in description of thermodynamical properties at low temperatures, and quantum effects should be accounted.

Fig. 2. Calculated magnetic part in molar heat capacity for various nickel chloride allotropes depending on the temperature: (1) the bulk NiCl2 (j) and fullerene (NiCl2)[email protected](NiCl2)3136 (+), (2) inﬁnite two-dimensional NiCl2 crystals and (3) NiCl2 nanostripes containing two, three and six NiCl2 layers (+, D, s, respectively), and (4) NiCl2 nanotubes with chiralities (44,44)@(50,50) (+), (38,38)@(44,44)@(50,50) (D) and (20,20)@(26,26)@(32,32)@(38,38)@(44,44)@(50,50) (s).

A.N. Enyashin, A.L. Ivanovskii / Computational Materials Science 49 (2010) 782–786

785

Fig. 3. Snapshots of spin ordering in the bulk NiCl2 and six-walled NiCl2 nanotube (20,20)@(26,26)@(32,32)@(38,38)@(44,44)@(50,50) at different temperatures.

Simulations for two-dimensional crystals of NiCl2 (the stacks composed by two, three and four of inﬁnite NiCl2 layers) reveal that antiferromagnetic ordering for such systems is preserved. The dependence of Cv on T also have a pronounced peak near 60 K (Fig. 2). However, the values TN comparing with that of the bulk crystal are lower. For example, TN for NiCl2 double layer is decreased on 6 K comparing to the bulk (Table 1). This phenomenon can be explained by the absence of a part of interaction of the surface spins – antiferromagnetic coupling with the spins of adjacent layer, which facilitates their easier disordering at the temperature growth. With increasing of the number of layers, the TN values of two-dimensional NiCl2 approach the TN of the bulk. An easier ability for rotation of the surface spins and for their easier disordering can be supported by the calculations of the energies of spin ordering DE (Table 1), which also decrease when the number of layers increases. Similar behavior is observed for one-dimensional planar nanostripes of NiCl2 (Fig. 2). All nanostripes keep antiferromagnetic ordering, but their Néel temperatures become lower comparing even to the inﬁnite two-dimensional crystals with corresponding number of the layers (Table 1). This decreasing TN can be explained by the presence of the spins at the edges of nanostripes, which have smaller coordination number, therefore, a weaker ferromagnetic coupling with the spins within the same layer. Thus, simple nanosizing does not change considerably antiferromagnetic properties of NiCl2, but causes their slight decaying – Table 1 Néel temperatures TN and relative energy of spin ordering DE within the bulk and nanostructured NiCl2 depending on the dimensionality D and morphology.a

a

System

D

TN (K)

DE (K/spin)

Bulk Inﬁnite double layer Inﬁnite triple layer Inﬁnite six layers Doublelayered nanostripe Triplelayered nanostripe Six-layered nanostripe [email protected] nanotube [email protected] nanotube [email protected]@50 nanotube [email protected]@[email protected] nanotube [email protected]@[email protected]@[email protected] nanotube (NiCl2)[email protected](NiCl2)3136 fullerene

3 2 2 2 1 1 1 1 1 1 1 1 0

63 57 60 61 55 58 61 61 62 65 66 69 68

0 3.11 2.34 1.57 4.37 3.67 2.92 0.26 0.37 2.15 3.07 4.06 7.07

All nanotubes considered are of armchair chirality, only one index is indicated.

owing to an easier ability for rotation of the ‘‘surface” spins for two-dimensional NiCl2 or for both ‘‘surface” and edges’ spins of NiCl2 nanostripes. One may expect that this decaying can be partially prevented in the case of closed multiwalled nanostructures (such as coaxial nanotubes and fullerenes), since they would not posses the edges with the atoms of low coordination number like in nanostripes. However, these low-dimensional nanostructures have different number of spins in adjacent walls, i.e., the number of spins in one layer is not compensated by the spins of a neighboring layer. The inﬂuence of this genuine feature of multiwalled inorganic nanostructures is not evident a priori. The results for MC simulations of magnetic ordering within multi-walled nanotubes are depicted in Figs. 2 and 3 and listed in Table 1. All nanotubes have the dependences of Cv on T, which are typical for above considered antiferromagnetics NiCl2 structures. Though, already for double-walled NiCl2 nanotubes no remarkable decrease in TN comparing to the bulk is observed – as against of nanostripes or two-dimensional crystals. For example, maximal deviation (from the bulk) DTN = 2 K was found for double-walled (20,20)@(26,26) nanotube, which is less than for a double-walled nanostripe with DTN = 8 K. Moreover, the nanotubes with number of wall more than two demonstrate even an increase TN on a few Ks (Table 1). High values of TN for multi-walled NiCl2 nanotubes comparing with that of the bulk also correlate with relative energies of spin ordering DE (Table 1). In these cases they have negative values evidencing about stronger coupling of the spins. Antiferromagnetic ordering of spins within the walls of multi-walled NiCl2 nanotubes is preserved until temperatures TN and no special feature was found in comparison with that of the bulk crystal (Fig. 3). Finally, according to our simulations (Fig. 2), zero-dimensional double-walled fullerene (NiCl2)[email protected](NiCl2)3136 is also an antiferromagnetic particle (Fig. 2.1). Like for NiCl2 nanotubes a shift of TN in the area of higher temperatures and negative energy of spin ordering are found (Table 1).

4. Conclusions Many properties of the solids undergo a considerable change or novel ones appear, when the size of particles is reduced. A special interest is given to the research of ferromagnetic properties of irongroup metal nanoparticles as materials for high-density recording

786

A.N. Enyashin, A.L. Ivanovskii / Computational Materials Science 49 (2010) 782–786

[23]. Under certain limit the magnetic moment of these nanoparticles becomes unstable, and these nanoparticles acquire superparamagnetism. This process unwanted for applied purposes can be beat up using magnetic exchange coupling induced at the interface between ferromagnetic and antiferromagnetic systems [24]. However, a change of antiferromagnetic properties due to a nanosizing could be also possible, which can prevent the usage of exchange bias. Among antiferromagnetic materials suitable for a range of practical applications d-metals dihalides attract a valuable interest. In this work atomic models of a set of low-dimensional NiCl2 nanostructures – multilayered nanostripes, nanotubes and a fullerene – were constructed. Together with the bulk and two-dimensional crystals of NiCl2 they were used to study an inﬂuence of dimensionality and morphology type on magnetic properties of NiCl2 – a classical layered antiferromagnetic system. Our results show that, all nanostructures considered remain antiferromagnetic. For planar two-dimensional NiCl2 crystals and one-dimensional nanostripes antiferromagnetic state becomes less favorable, and the values of Néel temperature TN are shifted down comparing to that of the bulk. On the contrary, for curved and closed nanostructures – multi-walled nanotubes and fullerenes – a gain in energy of spin ordering testiﬁes about slightly stronger spin interaction. Magnetic disordering in these hollow low-dimensional nanostructures appears at higher TN, than for the bulk. Hence, a nanostructuring at the size reducing can have a propitious inﬂuence on the preservation of antiferromagnetic properties and the suppression of superparamagnetic limit. Acknowledgement The authors are grateful to the Russian Foundation for Basic Research (Grant 10-03-96004-Ural).

References [1] L. Landau, Phys. Z. Sowjietunion 4 (1933) 675. [2] R.H. Busey, W.F. Giauque, J. Am. Chem. Soc. 6 (1952) 4443. [3] A.P. Lingård, R.J. Birgeneau, J. Als-Nielsen, H.J. Guggenheim, J. Phys. C 8 (1075) 1059. [4] D. Billerey, C. Terrier, A.J. Pointon, J.P. Redoules, J. Magn. Magn. Mater. 21 (1980) 187. [5] Y.R. Hacohen, E. Grunbaum, R. Tenne, J. Sloan, J.L. Hutchison, Nature 395 (1998) 336. [6] Y.R. Hacohen, R. Popovitz-Biro, E. Grunbaum, Y. Prior, R. Tenne, Adv. Mater. 14 (2002) 1075. [7] Y.R. Hacohen, R. Popovitz-Biro, Y. Prior, S. Gemming, G. Seifert, R. Tenne, Phys. Chem. Chem. Phys. 5 (2003) 1644. [8] R. Popovitz-Biro, A. Twersky, Y.R. Hacohen, R. Tenne, Israel J. Chem. 7 (2001) 41. [9] R. Popovitz-Biro, N. Sallacan, R. Tenne, J. Mater. Chem. 13 (2003) 1631. [10] N. Sallacan, R. Popovitz-Biro, R. Tenne, Solid State Sci. 5 (2003) 905. [11] M. Bar-Sadan, R. Popovitz-Biro, Y. Prior, R. Tenne, Mater. Res. Bull. 41 (2006) 2137. [12] R. Kreizman, S. Hong, J. Sloan, R. Popovitz-Biro, A. Albu-Yaron, G. Tobias, B. Ballesteros, B.G. Davis, M.L.H. Green, R. Tenne, Angew. Chem. Int. Ed. 47 (2008) 1. [13] A.N. Enyashin, R. Kreizman, R. Tenne, J. Phys. Chem. C 113 (2009) 13664. [14] G. Seifert, H. Terrones, M. Terrones, G. Jungnickel, T. Frauenheim, Phys. Rev. Lett. 85 (2000) 146. [15] R. Kreizman, A.N. Enyashin, F. Deepak, A. Albu-Yaron, R. Popovitz-Biro, G. Seifert, R. Tenne R, Adv. Funct. Mater. doi:10.1002/adfm. [16] A. Zak, L. Sallacan-Ecker, A. Margolin, M. Genut, R. Tenne, Nano 4 (2009) 91. [17] A. Ferrari, A. Braibanti, G. Bigliardi, Acta Cryst. 16 (1963) 846. [18] A.L. Ivanovskii, Uspekhi Khimii 71 (2002) 203. [19] R. Tenne, M. Remškar, A. Enyashin, G. Seifert, Topics Appl. Phys. 111 (2010) 631. [20] A.N. Enyashin, S. Gemming, M. Bar-Sadan, R. Popovitz-Biro, S.Y. Hong, Y. Prior, R. Tenne, G. Seifert, Angew. Chem. Int. Ed. 46 (2007) 623. [21] A.N. Enyashin, G. Seifert, Phys. Chem. Chem. Phys. 9 (2007) 5772. [22] N. Metropolis, A.W. Rosenbluth, M.N. Rosenbluth, A.H. Teller, E. Teller, J. Chem. Phys. 21 (1953) 1087. [23] J. Nogués, J. Sort, V. Langlais, V. Skumryev, S. Suriñach, J. Muñoz, M.D. Baró, Phys. Rep. 422 (2005) 65. [24] V. Skumryev, S. Stoyanov, Y. Zhang, G. Hadjipanayis, D. Givord, J. Nogués, Nature 423 (2003) 850.

Copyright © 2021 COEK.INFO. All rights reserved.